Tensile Test Ontology (TTO) data mapping example
type: Ontology
creator: Jörg Waitelonis
creator: Bernd Bayerlein
creator: Markus Schilling
creator: Philipp von Hartrott
imports: tto
version info: 2.0.0

process/pmdao-tto-tt-S355-9testpiece_id/Zd2
type: Table
type: Dataset
format: text/csv
table schema: Zd2 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zd2.csv

Zd2 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-10testpiece_id/Zd3
type: Table
type: Dataset
format: text/csv
table schema: Zd3 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zd3.csv

Zd3 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-1testpiece_id/Zx1
type: Table
type: Dataset
format: text/csv
table schema: Zx1 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zx1.csv

Zx1 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-2testpiece_id/Zx2
type: Table
type: Dataset
format: text/csv
table schema: Zx2 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zx2.csv

Zx2 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-3testpiece_id/Zx3
type: Table
type: Dataset
format: text/csv
table schema: Zx3 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zx3.csv

Zx3 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-4testpiece_id/Zx4
type: Table
type: Dataset
format: text/csv
table schema: Zx4 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zx4.csv

Zx4 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-5testpiece_id/Zy1
type: Table
type: Dataset
format: text/csv
table schema: Zy1 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zy1.csv

Zy1 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-6testpiece_id/Zy2
type: Table
type: Dataset
format: text/csv
table schema: Zy2 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zy2.csv

Zy2 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-7testpiece_id/Zy3
type: Table
type: Dataset
format: text/csv
table schema: Zy3 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zy3.csv

Zy3 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

process/pmdao-tto-tt-S355-8testpiece_id/Zy4
type: Table
type: Dataset
format: text/csv
table schema: Zy4 schema
url: https://raw.githubusercontent.com/materialdigital/application-ontologies/d8ab894df5d56d3362cedb18c2b482da0836e959/tensile_test_ontology_TTO/data/primary_data/Zy4.csv

Zy4 schema
type: Schema
column: Time
  type: Column
  type: Duration
  datatype: 1
  header count: 2
  name: Time
  unit: SEC
column: Crosshead Separation
  type: Column
  type: CrossheadSeparation
  datatype: 2
  header count: 2
  name: Crosshead travel
  unit: MilliM
column: Force
  type: Column
  datatype: 3
  header count: 2
  name: Force
  unit: KiloN
column: Percentage Extension
  type: Column
  type: PercentageExtension
  datatype: 4
  header count: 2
  name: Strain
  unit: PERCENT

caliperManufacturer Orion
type: Manufacturer
type: Metadata
value: Orion

caliperSerialNumber AK807114
type: Metadata
type: NodeSerialNumber
value: AK807114

caliperSerialNumber BA606983
type: Metadata
type: NodeSerialNumber
value: BA606983

extensometerName
type: Metadata
type: NodeName
value: HBM

https://w3id.org/pmd/resource/_extensometerSerialNumber_28023/28024
type: Metadata
type: NodeSerialNumber
value: 28023/28024

https://w3id.org/pmd/resource/_extensometerSerialNumber_28323/28324
type: Metadata
type: NodeSerialNumber
value: 28323/28324

extensometerStandard
type: Metadata
type: Norm
value: DIN EN ISO 17025

institute BAM address
type: Address
type: Metadata
value: Unter den Eichen 87. 12205 Berlin

loadCellMaxForce 100
type: LoadCellCapacity
type: Metadata
unit: PERCENT
value: 100

Berlin
type: Location
type: Metadata

machineManufacturer
type: Manufacturer
type: Metadata
value: Instron

machineName
type: Metadata
type: NodeName
value: Maschine 1

machineSerialNumber h2486
type: Metadata
type: NodeSerialNumber
value: h2486

machineStandard
type: Metadata
type: Norm
value: DIN EN ISO 7500-1:2018, DIN EN ISO 9513

machineType 4505
type: Metadata
type: NodeType
value: 4505

micrometerGaugeManufacturer Orion
type: Manufacturer
type: Metadata
value: Orion

pmdao-tto-tt-S355-1
type: ProcessIdentifier
value: pmdao-tto-tt-S355-1

pmdao-tto-tt-S355-10
type: ProcessIdentifier
value: pmdao-tto-tt-S355-10

pmdao-tto-tt-S355-10 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.707

pmdao-tto-tt-S355-10 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 43.924

pmdao-tto-tt-S355-10 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.867

pmdao-tto-tt-S355-10 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.544

pmdao-tto-tt-S355-10 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.71

pmdao-tto-tt-S355-10 date
type: Date
type: Metadata
value: 20.12.2021

pmdao-tto-tt-S355-10 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-10 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-10 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 79.97

pmdao-tto-tt-S355-10 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-10 note
type: Metadata
type: Note
value: Proben aus Stahlblech entnommen, diagonal der Walzrichtung

pmdao-tto-tt-S355-10 operator
type: Metadata
type: Operator
value: M./S./G.

pmdao-tto-tt-S355-10 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-10 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-10 rollingDirection
type: MaterialRelated
type: Metadata
value: diagonal to rolling direction

pmdao-tto-tt-S355-10 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-10 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-10 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.16

pmdao-tto-tt-S355-10 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.993

pmdao-tto-tt-S355-10 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.985

pmdao-tto-tt-S355-10 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.99

pmdao-tto-tt-S355-10 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 4.0

pmdao-tto-tt-S355-10 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 13.9

pmdao-tto-tt-S355-10 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.168

pmdao-tto-tt-S355-10 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.141

pmdao-tto-tt-S355-10 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.152

pmdao-tto-tt-S355-1 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.636

pmdao-tto-tt-S355-1 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 52.659

pmdao-tto-tt-S355-1 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.675

pmdao-tto-tt-S355-1 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.608

pmdao-tto-tt-S355-1 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.625

pmdao-tto-tt-S355-1 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-1 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-1 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-1 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: NaN

pmdao-tto-tt-S355-1 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-1 note
type: Metadata
type: Note
value: In Walzrichtung aus Stahlblech entnommen; Abweichend von den anderen Proben. Weggeschwindigkeit wurde erhöht.

pmdao-tto-tt-S355-1 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-1 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-1 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-1 rollingDirection
type: MaterialRelated
type: Metadata
value: in rolling direction

pmdao-tto-tt-S355-1 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-1 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-1 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.52

pmdao-tto-tt-S355-1 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.993

pmdao-tto-tt-S355-1 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.987

pmdao-tto-tt-S355-1 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.992

pmdao-tto-tt-S355-1 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 1.6

pmdao-tto-tt-S355-1 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.96

pmdao-tto-tt-S355-1 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.136

pmdao-tto-tt-S355-1 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.145

pmdao-tto-tt-S355-1 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.131

pmdao-tto-tt-S355-2
type: ProcessIdentifier
value: pmdao-tto-tt-S355-2

pmdao-tto-tt-S355-2 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.444

pmdao-tto-tt-S355-2 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 49.585

pmdao-tto-tt-S355-2 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.503

pmdao-tto-tt-S355-2 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.425

pmdao-tto-tt-S355-2 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.403

pmdao-tto-tt-S355-2 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-2 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-2 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-2 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 81.0

pmdao-tto-tt-S355-2 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-2 note
type: Metadata
type: Note
value: In Walzrichtung aus Stahlblech entnommen; Extensometer nach 3,9 % Dehnung der Proben entfernt. Keine Erhöhung der Geschwindigkeit.

pmdao-tto-tt-S355-2 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-2 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-2 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-2 rollingDirection
type: MaterialRelated
type: Metadata
value: in rolling direction

pmdao-tto-tt-S355-2 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-2 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-2 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.38

pmdao-tto-tt-S355-2 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.991

pmdao-tto-tt-S355-2 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.991

pmdao-tto-tt-S355-2 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.992

pmdao-tto-tt-S355-2 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 3.8

pmdao-tto-tt-S355-2 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.67

pmdao-tto-tt-S355-2 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.114

pmdao-tto-tt-S355-2 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.101

pmdao-tto-tt-S355-2 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.094

pmdao-tto-tt-S355-3
type: ProcessIdentifier
value: pmdao-tto-tt-S355-3

pmdao-tto-tt-S355-3 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.396

pmdao-tto-tt-S355-3 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 50.502

pmdao-tto-tt-S355-3 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.323

pmdao-tto-tt-S355-3 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.431

pmdao-tto-tt-S355-3 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.433

pmdao-tto-tt-S355-3 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-3 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-3 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-3 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 81.1

pmdao-tto-tt-S355-3 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-3 note
type: Metadata
type: Note
value: In Walzrichtung aus Stahlblech entnommen; Extensometer nach 3,9 % Dehnung der Proben entfernt. Keine Erhöhung der Geschwindigkeit.

pmdao-tto-tt-S355-3 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-3 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-3 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-3 rollingDirection
type: MaterialRelated
type: Metadata
value: in rolling direction

pmdao-tto-tt-S355-3 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-3 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-3 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.41

pmdao-tto-tt-S355-3 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.991

pmdao-tto-tt-S355-3 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.994

pmdao-tto-tt-S355-3 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.992

pmdao-tto-tt-S355-3 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 3.8

pmdao-tto-tt-S355-3 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.81

pmdao-tto-tt-S355-3 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.084

pmdao-tto-tt-S355-3 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.092

pmdao-tto-tt-S355-3 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.099

pmdao-tto-tt-S355-4
type: ProcessIdentifier
value: pmdao-tto-tt-S355-4

pmdao-tto-tt-S355-4 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.014

pmdao-tto-tt-S355-4 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 47.382

pmdao-tto-tt-S355-4 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.095

pmdao-tto-tt-S355-4 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 119.99

pmdao-tto-tt-S355-4 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 119.958

pmdao-tto-tt-S355-4 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-4 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-4 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-4 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 80.9

pmdao-tto-tt-S355-4 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-4 note
type: Metadata
type: Note
value: In Walzrichtung aus Stahlblech entnommen; Extensometer nach 3,9 % Dehnung der Proben entfernt. Keine Erhöhung der Geschwindigkeit.

pmdao-tto-tt-S355-4 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-4 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-4 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-4 rollingDirection
type: MaterialRelated
type: Metadata
value: in rolling direction

pmdao-tto-tt-S355-4 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-4 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-4 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.27

pmdao-tto-tt-S355-4 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.982

pmdao-tto-tt-S355-4 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.978

pmdao-tto-tt-S355-4 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.977

pmdao-tto-tt-S355-4 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 3.8

pmdao-tto-tt-S355-4 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.49

pmdao-tto-tt-S355-4 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.076

pmdao-tto-tt-S355-4 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.072

pmdao-tto-tt-S355-4 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 45.127

pmdao-tto-tt-S355-5
type: ProcessIdentifier
value: pmdao-tto-tt-S355-5

pmdao-tto-tt-S355-5 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.679

pmdao-tto-tt-S355-5 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 56.039

pmdao-tto-tt-S355-5 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.774

pmdao-tto-tt-S355-5 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.637

pmdao-tto-tt-S355-5 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.627

pmdao-tto-tt-S355-5 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-5 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-5 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-5 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: NaN

pmdao-tto-tt-S355-5 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-5 note
type: Metadata
type: Note
value: Proben aus Stahlblech entnommen, entgegen der Walzrichtung

pmdao-tto-tt-S355-5 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-5 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-5 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-5 rollingDirection
type: MaterialRelated
type: Metadata
value: perpendicular to rolling direction

pmdao-tto-tt-S355-5 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-5 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-5 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.82

pmdao-tto-tt-S355-5 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 6.0

pmdao-tto-tt-S355-5 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.992

pmdao-tto-tt-S355-5 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.993

pmdao-tto-tt-S355-5 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 3.8

pmdao-tto-tt-S355-5 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.67

pmdao-tto-tt-S355-5 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.129

pmdao-tto-tt-S355-5 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.133

pmdao-tto-tt-S355-5 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.128

pmdao-tto-tt-S355-6
type: ProcessIdentifier
value: pmdao-tto-tt-S355-6

pmdao-tto-tt-S355-6 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.71

pmdao-tto-tt-S355-6 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 53.435

pmdao-tto-tt-S355-6 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.765

pmdao-tto-tt-S355-6 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.6

pmdao-tto-tt-S355-6 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.764

pmdao-tto-tt-S355-6 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-6 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-6 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-6 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 81.0

pmdao-tto-tt-S355-6 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-6 note
type: Metadata
type: Note
value: Proben aus Stahlblech entnommen, entgegen der Walzrichtung

pmdao-tto-tt-S355-6 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-6 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-6 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-6 rollingDirection
type: MaterialRelated
type: Metadata
value: perpendicular to rolling direction

pmdao-tto-tt-S355-6 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-6 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-6 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.64

pmdao-tto-tt-S355-6 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.996

pmdao-tto-tt-S355-6 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.989

pmdao-tto-tt-S355-6 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.998

pmdao-tto-tt-S355-6 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 3.8

pmdao-tto-tt-S355-6 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.68

pmdao-tto-tt-S355-6 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.141

pmdao-tto-tt-S355-6 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.137

pmdao-tto-tt-S355-6 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.134

pmdao-tto-tt-S355-7
type: ProcessIdentifier
value: pmdao-tto-tt-S355-7

pmdao-tto-tt-S355-7 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.663

pmdao-tto-tt-S355-7 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 50.365

pmdao-tto-tt-S355-7 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.581

pmdao-tto-tt-S355-7 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.581

pmdao-tto-tt-S355-7 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.826

pmdao-tto-tt-S355-7 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-7 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-7 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-7 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 80.14

pmdao-tto-tt-S355-7 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-7 note
type: Metadata
type: Note
value: Proben aus Stahlblech entnommen, entgegen der Walzrichtung

pmdao-tto-tt-S355-7 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-7 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-7 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-7 rollingDirection
type: MaterialRelated
type: Metadata
value: perpendicular to rolling direction

pmdao-tto-tt-S355-7 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-7 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-7 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.5

pmdao-tto-tt-S355-7 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.991

pmdao-tto-tt-S355-7 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.991

pmdao-tto-tt-S355-7 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 6.002

pmdao-tto-tt-S355-7 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 3.8

pmdao-tto-tt-S355-7 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.39

pmdao-tto-tt-S355-7 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.127

pmdao-tto-tt-S355-7 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.127

pmdao-tto-tt-S355-7 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.131

pmdao-tto-tt-S355-8
type: ProcessIdentifier
value: pmdao-tto-tt-S355-8

pmdao-tto-tt-S355-8 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.583

pmdao-tto-tt-S355-8 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 54.132

pmdao-tto-tt-S355-8 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.561

pmdao-tto-tt-S355-8 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.501

pmdao-tto-tt-S355-8 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.687

pmdao-tto-tt-S355-8 date
type: Date
type: Metadata
value: 22.02.2021

pmdao-tto-tt-S355-8 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-8 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-8 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 79.74

pmdao-tto-tt-S355-8 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-8 note
type: Metadata
type: Note
value: Proben aus Stahlblech entnommen, entgegen der Walzrichtung

pmdao-tto-tt-S355-8 operator
type: Metadata
type: Operator
value: M. (S., J.)

pmdao-tto-tt-S355-8 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-8 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-8 rollingDirection
type: MaterialRelated
type: Metadata
value: perpendicular to rolling direction

pmdao-tto-tt-S355-8 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-8 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-8 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.69

pmdao-tto-tt-S355-8 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.982

pmdao-tto-tt-S355-8 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.979

pmdao-tto-tt-S355-8 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.99

pmdao-tto-tt-S355-8 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 3.8

pmdao-tto-tt-S355-8 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 14.67

pmdao-tto-tt-S355-8 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.154

pmdao-tto-tt-S355-8 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.154

pmdao-tto-tt-S355-8 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.148

pmdao-tto-tt-S355-9
type: ProcessIdentifier
value: pmdao-tto-tt-S355-9

pmdao-tto-tt-S355-9 crossSectionArea S0
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.715

pmdao-tto-tt-S355-9 crossSectionArea Su
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 48.813

pmdao-tto-tt-S355-9 crossSectionArea s1
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.649

pmdao-tto-tt-S355-9 crossSectionArea s2
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.683

pmdao-tto-tt-S355-9 crossSectionArea s3
type: CrossSectionArea
type: Measurement
type: PrimaryData
unit: MilliM2
value: 120.813

pmdao-tto-tt-S355-9 date
type: Date
type: Metadata
value: 20.12.2021

pmdao-tto-tt-S355-9 environmentalTemperature
type: EnvironmentalTemperature
type: Measurement
type: Metadata
unit: DEG C
value: 20

pmdao-tto-tt-S355-9 extensometerGaugeLength
type: Measurement
type: Metadata
type: ExtensometerGaugeLength
unit: MilliM
value: 50

pmdao-tto-tt-S355-9 finalGaugeLengthAfterFracture Lu
type: Measurement
type: PrimaryData
type: FinalGaugeLengthAfterFracture
unit: MilliM
value: 80.02

pmdao-tto-tt-S355-9 materialDescription
type: Metadata
type: materialDesignation
value: S355

pmdao-tto-tt-S355-9 note
type: Metadata
type: Note
value: Proben aus Stahlblech entnommen, diagonal der Walzrichtung

pmdao-tto-tt-S355-9 operator
type: Metadata
type: Operator
value: M./S./G.

pmdao-tto-tt-S355-9 originalGaugeLength L0
type: Measurement
type: PrimaryData
type: OriginalGaugeLength
unit: MilliM
value: 60

pmdao-tto-tt-S355-9 project ID
type: Metadata
type: ProjectIdentifier
value: PMDao-onto_1

pmdao-tto-tt-S355-9 rollingDirection
type: MaterialRelated
type: Metadata
value: diagonal to rolling direction

pmdao-tto-tt-S355-9 specimenShape
type: Metadata
type: GeometryShape
value: E6x20x60

pmdao-tto-tt-S355-9 strainRate
type: Metadata
type: SetPoint
type: StrainRate
value: 0.00025

pmdao-tto-tt-S355-9 thicknessAfterFracture au
type: Measurement
type: PrimaryData
type: ThicknessAfterFracture
unit: MilliM
value: 3.55

pmdao-tto-tt-S355-9 thickness a1
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.992

pmdao-tto-tt-S355-9 thickness a2
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.991

pmdao-tto-tt-S355-9 thickness a3
type: Measurement
type: PrimaryData
type: OriginalThickness
unit: MilliM
value: 5.993

pmdao-tto-tt-S355-9 transitionPoint
type: Metadata
type: SetPoint
type: TransitionPointTestingRate
unit: PERCENT
value: 4.0

pmdao-tto-tt-S355-9 widthAfterFracture bu
type: Measurement
type: PrimaryData
type: WidthAfterFracture
unit: MilliM
value: 13.75

pmdao-tto-tt-S355-9 width b1
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.135

pmdao-tto-tt-S355-9 width b2
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.144

pmdao-tto-tt-S355-9 width b3
type: Measurement
type: PrimaryData
type: OriginalWidth
unit: MilliM
value: 20.159

Zd2
type: Metadata
type: TestPieceName
value: Zd2

Zd2 afterTest 1
type: Metadata
type: TestPieceName
value: Zd2_afterTest_1

Zd2 afterTest 2
type: Metadata
type: TestPieceName
value: Zd2_afterTest_2

Zd3
type: Metadata
type: TestPieceName
value: Zd3

Zd3 afterTest 1
type: Metadata
type: TestPieceName
value: Zd3_afterTest_1

Zd3 afterTest 2
type: Metadata
type: TestPieceName
value: Zd3_afterTest_2

Zx1
type: Metadata
type: TestPieceName
value: Zx1

Zx1 afterTest 1
type: Metadata
type: TestPieceName
value: Zx1_afterTest_1

Zx1 afterTest 2
type: Metadata
type: TestPieceName
value: Zx1_afterTest_2

Zx2
type: Metadata
type: TestPieceName
value: Zx2

Zx2 afterTest 1
type: Metadata
type: TestPieceName
value: Zx2_afterTest_1

Zx2 afterTest 2
type: Metadata
type: TestPieceName
value: Zx2_afterTest_2

Zx3
type: Metadata
type: TestPieceName
value: Zx3

Zx3 afterTest 1
type: Metadata
type: TestPieceName
value: Zx3_afterTest_1

Zx3 afterTest 2
type: Metadata
type: TestPieceName
value: Zx3_afterTest_2

Zx4
type: Metadata
type: TestPieceName
value: Zx4

Zx4 afterTest 1
type: Metadata
type: TestPieceName
value: Zx4_afterTest_1

Zx4 afterTest 2
type: Metadata
type: TestPieceName
value: Zx4_afterTest_2

Zy1
type: Metadata
type: TestPieceName
value: Zy1

Zy1 afterTest 1
type: Metadata
type: TestPieceName
value: Zy1_afterTest_1

Zy1 afterTest 2
type: Metadata
type: TestPieceName
value: Zy1_afterTest_2

Zy2
type: Metadata
type: TestPieceName
value: Zy2

Zy2 afterTest 1
type: Metadata
type: TestPieceName
value: Zy2_afterTest_1

Zy2 afterTest 2
type: Metadata
type: TestPieceName
value: Zy2_afterTest_2

Zy3
type: Metadata
type: TestPieceName
value: Zy3

Zy3 afterTest 1
type: Metadata
type: TestPieceName
value: Zy3_afterTest_1

Zy3 afterTest 2
type: Metadata
type: TestPieceName
value: Zy3_afterTest_2

Zy4
type: Metadata
type: TestPieceName
value: Zy4

Zy4 afterTest 1
type: Metadata
type: TestPieceName
value: Zy4_afterTest_1

Zy4 afterTest 2
type: Metadata
type: TestPieceName
value: Zy4_afterTest_2

pmdao-tto-tt-S355-10 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 61.681

pmdao-tto-tt-S355-10 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 195

pmdao-tto-tt-S355-10 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 33.0

pmdao-tto-tt-S355-10 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 64

pmdao-tto-tt-S355-10 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: NaN

pmdao-tto-tt-S355-10 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 511

pmdao-tto-tt-S355-10 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 396

pmdao-tto-tt-S355-1 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 62.007

pmdao-tto-tt-S355-1 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 194

pmdao-tto-tt-S355-1 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: NaN

pmdao-tto-tt-S355-1 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 56

pmdao-tto-tt-S355-1 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 375.0

pmdao-tto-tt-S355-1 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 514

pmdao-tto-tt-S355-1 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 380

pmdao-tto-tt-S355-2 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 60.704

pmdao-tto-tt-S355-2 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 199

pmdao-tto-tt-S355-2 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 35.0

pmdao-tto-tt-S355-2 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 59

pmdao-tto-tt-S355-2 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 374.0

pmdao-tto-tt-S355-2 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 504

pmdao-tto-tt-S355-2 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 379

pmdao-tto-tt-S355-3 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 60.68

pmdao-tto-tt-S355-3 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 199

pmdao-tto-tt-S355-3 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 35.0

pmdao-tto-tt-S355-3 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 58

pmdao-tto-tt-S355-3 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 376.0

pmdao-tto-tt-S355-3 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 504

pmdao-tto-tt-S355-3 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 379

pmdao-tto-tt-S355-4 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 62.288

pmdao-tto-tt-S355-4 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 196

pmdao-tto-tt-S355-4 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 35.0

pmdao-tto-tt-S355-4 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 61

pmdao-tto-tt-S355-4 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 382.0

pmdao-tto-tt-S355-4 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 519

pmdao-tto-tt-S355-4 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 388

pmdao-tto-tt-S355-5 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 61.305

pmdao-tto-tt-S355-5 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 210

pmdao-tto-tt-S355-5 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: NaN

pmdao-tto-tt-S355-5 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 54

pmdao-tto-tt-S355-5 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 396.0

pmdao-tto-tt-S355-5 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 508

pmdao-tto-tt-S355-5 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 399

pmdao-tto-tt-S355-6 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 61.2

pmdao-tto-tt-S355-6 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 214

pmdao-tto-tt-S355-6 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 35.0

pmdao-tto-tt-S355-6 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 56

pmdao-tto-tt-S355-6 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 390.0

pmdao-tto-tt-S355-6 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 507

pmdao-tto-tt-S355-6 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 399

pmdao-tto-tt-S355-7 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 60.935

pmdao-tto-tt-S355-7 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 206

pmdao-tto-tt-S355-7 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 33.5

pmdao-tto-tt-S355-7 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 58

pmdao-tto-tt-S355-7 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: NaN

pmdao-tto-tt-S355-7 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 505

pmdao-tto-tt-S355-7 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 408

pmdao-tto-tt-S355-8 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 61.98

pmdao-tto-tt-S355-8 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 211

pmdao-tto-tt-S355-8 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 33.0

pmdao-tto-tt-S355-8 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 55

pmdao-tto-tt-S355-8 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 402.0

pmdao-tto-tt-S355-8 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 514

pmdao-tto-tt-S355-8 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 407

pmdao-tto-tt-S355-9 maximumForce
type: Measurement
type: SecondaryData
type: MaximumForce
unit: kiloN
value: 62.168

pmdao-tto-tt-S355-9 modulusOfElasticity
type: Measurement
type: ModulusOfElasticity
type: SecondaryData
type: SlopeOfTheElasticPart
unit: GigaPa
value: 201

pmdao-tto-tt-S355-9 percentageElongationAfterFracture
type: Measurement
type: SecondaryData
type: PercentageElongationAfterFracture
unit: PERCENT
value: 33.5

pmdao-tto-tt-S355-9 percentageReductionOfArea
type: Measurement
type: SecondaryData
type: PercentageReductionOfArea
unit: PERCENT
value: 60

pmdao-tto-tt-S355-9 proofStrength Rp02
type: Measurement
type: SecondaryData
type: Rp02
unit: MegaPa
value: 390.0

pmdao-tto-tt-S355-9 tensileStrength
type: Measurement
type: SecondaryData
type: TensileStrength
unit: MegaPa
value: 515

pmdao-tto-tt-S355-9 upperYieldStrength
type: Measurement
type: SecondaryData
type: UpperYieldStrength
unit: MegaPa
value: 399

Funder Identifier
type: FunderIdentifier
uses identifier scheme: local-funder-identifier-scheme
value: 13XP5094

Bundesministerium für Bildung und Forschung (BMBF)@de
type: OrganizationIdentifier
uses identifier scheme: Wikidata
alternative label: Federal Ministry of Education and Research@en
value: Q492234

Bundesanstalt für Materialforschung und -prüfung (BAM)
type: Organization
type: Metadata
characteristic: institute BAM address
characteristic: Berlin

software agent
type: SoftwareAgent
type: Metadata
value: BAM Tensile Test Analysis App

standard
type: Metadata
type: Norm
value: DIN EN ISO 6892-1